| ||Format||Pages||Price|| |
|9||$45.00||  ADD TO CART|
|Hardcopy (shipping and handling)||9||$45.00||  ADD TO CART|
|Standard + Redline PDF Bundle||18||$54.00||  ADD TO CART|
This specification deals with the standard requirements for untreated and heat-treated carbon and alloy steel forgings for general industrial use. This specification covers six classes of carbon steels (Class A to F) and seven classes of alloy steels (Class G, H, and J to N). Materials shall be forged by hot mechanical work. Except for Class A, all forgings shall be heat treated, depending on class, by the following techniques: annealed, or normalized, or normalized and tempered (Classes B, C, D, and G); normalized and tempered, or double-normalized and tempered (Class E); quenched and tempered, or normalized, quenched, and tempered (Classes F); normalized and tempered (Class H); normalized and tempered, or normalized, quenched, and tempered (Class J); and normalized, quenched, and tempered (Classes K, L, M, and N). Steel specimens shall undergo heat and product analyses, and shall conform to required chemical compositions for manganese, phosphorus, and sulfur. Steel forgings shall also be tested on their conformance to the following tensile requirements: tensile strength, yield point, yield strength, elongation, reduction of area, and Brinell hardness.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers untreated and heat-treated carbon and alloy steel forgings for general industrial use. Other ASTM specifications for forgings are available for specific applications such as pressure vessels, railroad use, turbine generators, gearing, and others involving special temperature requirements.
1.2 Hot-rolled or cold finished bars are not within the scope of this specification.
1.3 Six classes of carbon steel and seven classes of alloy steel forgings are listed (see Section ), which indicates their required heat treatments, as well as mechanical properties.
1.4 Provision, with the suffix H for certification and marking, for the supply of forgings after hardness testing only.
1.5 Supplementary requirements, including those in Specification , of an optional nature are provided. These shall apply only when specified by the purchaser.
1.6 lists the current classes corresponding to the various classes of Specifications , , and , which have been superseded by this specification.
1.7 The values stated in either SI units or inch-pound units are to be regarded separately as standard; within the text and tables, the SI units are shown in brackets. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in nonconformance with the standard.
1.8 Unless the order specifies the applicable "M" specification, the forgings shall be furnished to the inch-pound units.
ICS Number Code 77.140.85 (Iron and steel forgings)
UNSPSC Code 31132100(Steel forgings)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM A668 / A668M-16, Standard Specification for Steel Forgings, Carbon and Alloy, for General Industrial Use, ASTM International, West Conshohocken, PA, 2016, www.astm.orgBack to Top